12 glass ionomer cements as restorative and preventive materials
Glass-IonomerC e m e n t s asRestorative andP re v e n t i v e M a t e r i a l sHien Ngo, BDS, MDS, PhD, FADI, FICD, FPFA KEYWORDS Glass-ionomer cement Therapeutic coating Internal remineralisation CariesThis article will focus on glass-ionomer cement (GIC) and its role in the clinicalmanagement of caries. It begins with a brief description of GIC, the mechanism of fluo-ride release and ion exchange, the interaction between GIC and the external environ-ment, and finally the ion exchange between GIC and the tooth at the internal interface.The importance of GIC, as a tool, in caries management, in minimal interventiondentistry, and Caries Management by Risk Assessment (CAMBRA) also will behighlighted. The philosophy of minimal intervention density (MI) and the CAMBRA approach isgaining popularity worldwide as both integrate the new understanding that caries isa biofilm-related, multifactorial and lifestyle-associated bi-directional disease. Thereis now an acceptance that to manage caries disease effectively, it is important tomove from the surgical approach to a combined surgical—medical approach, withspecial focus on engaging patients in changing their lifestyle. The following statementis a consensus of 165 experts, comprising of clinicians, scientists, educators, andhealth service managers from 15 countries, who gathered in Bangkok for a consulta-tive meeting to discuss the MI philosophy (personal communication, 2009): ‘‘The current surgical model of caries management does not fully address the multi-factorial nature of dental caries. This model often results in unnecessary removal of tooth structure, can impact negatively on general health and quality of life and can impose substantial cost.’’ Glass-ionomer cement (GIC) is an important tool in the fight against caries. It can bethought of as a reservoir of fluoride and other ions in the oral cavity, a mechanicalbarrier that protects the tooth surface against bacteria; most importantly, it canprovide a long-lasting seal under the most challenging clinical circumstances. General Dental Practice, School of Dentistry, The University of Queensland, 200 Turbot Street, Brisbane, QLD 4000, Australia E-mail address: email@example.com Dent Clin N Am 54 (2010) 551–563 doi:10.1016/j.cden.2010.04.001 dental.theclinics.com 0011-8532/10/$ – see front matter ª 2010 Published by Elsevier Inc.
552 Ngo GIC is very versatile. It may be utilized as a definitive restorative material, a prepara- tion liner, a restorative base material, a luting cement, or a fissure sealant. Recently, it was suggested that GIC also could be useful in the preventive arena as therapeutic coating. This new terminology is utilized to describe a material that can be painted on a susceptible surface and form a long-lasting coat to protect, both mechanically and chemically, against accumulation of plaque where patients are unable to render effective hygiene in certain parts of the oral cavity. Clinical examples of these applica- tions will be given at the end of the article. HISTORICAL PERSPECTIVE There is a spectrum of tooth-colored restorative materials, spanning from GIC at one end to the resin-based materials at the other end. Wilson and McLean introduced the GIC family of materials to the dental profession in 1988.1 The four families of acid–base materials used in dentistry are: silicate, zinc phosphate, polycarboxylate, and glass- ionomer. They all utilize acid and base components (Table 1). It was over 100 years ago when silicate cements were introduced to dentistry as a restorative material. There was anecdotal evidence that silicate cements were an effective anticaries agent that was attributed mainly to the high level of fluoride release from the silicate material. The material’s solubility was high, however, and the search for its replacement led to the development of polycarboxylate cements, and eventually GIC. Currently, glass- ionomer is the only restorative material that is water-based and like silicate has an anti- caries effect.2–4 Current esthetic high-strength GICs are considered to be durable restorative dental cements.5 HOW DO GIC ACQUIRE THEIR ANTICARIES EFFECT? GICs are true acid–base cements where the base is the fluoroaluminosilicate glass powder and the liquid containing acid comes from the polyalkenoic family. In some glass formulations, the F rich phase of the glass can be visible (Fig. 1) and physically distinct. Apart from the base and acid, the third major component is water, the major component of the liquid. The total water content of the set cement is somewhere between 11% and 24%. Being a true water-based material, GIC also is recognized as the only biological active restorative material that is currently available.6 The precise glass composition varies from one material to another. Traditionally, GIC powder was based on calcium (Ca); however, there are several materials where the calcium has been substituted by strontium (Sr). This was done to impart radiopac- ity to the material. It is interesting to note that because of their similarity in polarity and atomic size, these two elements are interchangeable in the composition of GIC as well as hydroxyapatite (HAP). Some of the Ca in HAP can be substituted with Sr without any significant disadvantage.7 It is interesting to note that, at a population level, there is some evidence to show that Sr has anticariogenic properties. Curzon reported on the caries-reducing effect of drinking water containing strontium. He noted a reduction Table 1 The acid and base components used in the various dental cements Acid-Base Cement Acid Base Silicate Calcium-fluoro-alumino-silicate Phosphoric acid Zinc Phosphate Zinc oxide Phosphoric acid Polycarboxylate Zinc oxide Polyalkenoic acid Glass-Ionomer Calcium-fluoro-alumino-silicate Polyalkenoic acid
Glass-Ionomer Cements 553Fig. 1. Scanning electron microscope view of a set GIC showing a reacted glass particle ina set cement. The three areas of interest are: the silica ion–depleted gel phase, the glasscore with its fluoride-rich phase (dense white droplets), and the matrix of the cement.The minor crack is an artifact.in DMFT in a population exposed to drinking water containing strontium.8 The impor-tance of this information will become apparent in the discussion of a study relating tothe internal remineralization technique, where both F and Sr from GIC were found tomigrate from GIC to the soften dentine left at the base of cavities. For restorative GIC, approximately 60% of the liquid is water, which plays an impor-tant role in the setting reaction and in the final structure of the set cement, as well ascontributing to the observed biocompatibility and the well known ionic exchange.Water allows the acid–base reaction to occur and the migration of the various ionsout of and into the matrix of the set cement. When the powder is brought into contactwith the liquid, the acidity allows the matrix-forming cations, Ca or Sr and Al, to leachout of the glass. These will cross-link with the polyalkenoic chains to form metal poly-acrylate salts, which form the matrix and solidify the mix.9MOISTURE CONTROL AND THE CLINICAL PERFORMANCE OF GICThe setting reaction of GIC is a two-phase process.6,10 In the first phase, immediatelyafter mixing, there is cross-linking of the poly-acid chains by either the Ca or Sr ions.This cross-linking during this first phase is not stable and can be easily affected byexcessive water loss or gain. Clinically, this means that the restoration must be pro-tected, against initial water contamination and desiccation, immediately after place-ment. In the second phase, within the solidified cement, the poly-acid chains arefurther cross-linked by trivalent Al ions. This second phase gives the materialincreased physical properties and reduced solubility. In the set GIC, water molecules can be classified as either loosely bound or tightlybound. As the material matures, the ratio between the loosely bound and tightly boundwater decreases, and the material will show increased in physical properties. This isimportant for two reasons. First, the loosely bound water is essential for ion releaseand uptake, and second, it is important to maintain the water balance right throughthe life of a GIC restoration. Early exposure to excess water during setting and desic-cation, at any stage, will lead to poor clinical performance.ION EXCHANGE BETWEEN GIC AND THE EXTERNAL ENVIRONMENTBecause of the combined effect of release and uptake of ions, GIC is a rich reservoir ofapatite forming ions such as fluoride, calcium, strontium, and phosphate. In the
554 Ngo aqueous environment of the oral cavity, these are released through an ion exchange process with the environment. There is a natural exchange between Sr and Ca ions.11 As Sr leaves the set cement, an equivalent number of Ca ions from saliva enter the matrix of the cement to maintain electrolytic balance (Fig. 2). Nicholson postulated that this leads to the hardening of the surface, and this was confirmed by Okada when it was found that the surface hardness of a GIC can increase by 39% after 40 days storage in natural saliva.11–13 This was demonstrated by immersing 24 hours-old buttons of strontium containing GICs in an artificial saliva solution, and then a distribu- tion map of Ca was acquired using electron probe micro analysis (EPMA), which clearly showed that Ca was exchanged for Sr in the matrix of the surface layer of the GIC buttons (see Fig. 2). It was postulated that the increase in surface hardness was related to the exchange of Sr by Ca in the matrix; however, the mechanism involved has not yet been identified. This phenomenon means that an exposure to Ca-rich saliva is beneficial to the long-term clinical performance of GIC. One of the major advantages of GIC is the long-term release of fluoride and other ions. This is characterized by an initial high peak that will decline rapidly to a lower level and sustained over a number of years.14 It has been shown that there is a topping-up effect15,16 with the material up-taking fluoride from external sources such as tooth- paste and topical fluoride gel. Wilson studied this over a period of 20 months and found that these species still were being released at the end of the experimental period, although at a diminished rate.17 This fluoride release also can suppress the acidogenicity of the biofilm.18 From the above observations and what is known about the importance of fluoride in the demineralization and remineralization process, one can understand the protective effect that GIC has on tooth structure in its immediate Fig. 2. An elemental distribution map showing Ca (purple) in the matrix of a Sr-based GIC that was stored in saliva for 7 days.
Glass-Ionomer Cements 555Fig. 3. Cumulative release of Sr, F, and Al into solution.vicinity.2 As the level of fluoride, and other ions, in GIC can be recharged, this class ofmaterial can be used as a reservoir for fluoride and may act as a slow F release device.GIC also can provide protection by the combined effect of mechanical and chemicalmeans. For example, GIC can be used successfully to protect fissures, and despitea lower retention rate than resin-based fissure sealants, there is evidence that itreduces caries incidence in permanent teeth.19 In addition, a long-term clinical trialreported an effective rate of 80.6%, and suggested traditional retention is not essentialfor caries prevention.20 This is probably due to the effect of the chemical protection thematerial provides, and the fact that GIC tends to fail cohesively, so there is alwaysa remaining layer on the surface, even when GIC is no longer clinically detectable. This ion exchange is not only restricted to fluoride. The essential elements in a GICinclude Ca, or Sr, Al, Si, and F. After the completion of the setting reaction, a portion ofthese ions is available for transfer from the matrix to the surrounding environment. Asshown in (Fig. 3), the level of release of Sr far exceeds that of F or Al ions. It is wellaccepted that the release is caused by an exchange process, so it is unlikely toadversely affect the clinical performance of the material. The following segment looks at some new clinical indications where the biocompat-ibility effect of GIC is important for clinical success.ION EXCHANGE BETWEEN GIC AND CARIOUS DENTINEThe term internal remineralization was introduced to describe the interaction betweenGIC and carious dentine, and to suggest that GIC is an essential tool in theFig. 4. Initial presentation with symptoms consistent with reversible pulpitis.
556 Ngo Fig. 5. Presentation during preparation for access. management of deep caries lesions in permanent teeth as it supplies apatite-forming ions to the partially demineralized dentine at the base of cavity. Since the time of GV Black, cavity, designs have been classified and standardized. Regardless of the size and extent of the original lesions, the final shape and dimen- sions of the prepared cavity were designed to accommodate the shortcomings of the early restorative materials. In the 1970s, the author was taught that removing caries meant accessing the soft dentine and removing it until the floor and the walls of the cavity were stain-free and hard. Anything that did not resemble sound dentine had to be removed. The objective was to ensure the elimination of all remaining micro- organisms, which led to many unnecessary pulp exposures. This approach was justi- fied at the time for the following reasons. First, any soft dentin left under the filling would lead to insufficient support and could be detrimental to the longevity of the restoration and second, any bacteria left under the filling was thought to be detri- mental to the pulp. The first suggestion that the profession should move away from this concept was proposed by Fusayama21 and then Massler.22 They both suggested that there were two layers in carious dentine. The outer layer was heavily infected by microorganisms and was broken down to the extent that it could not be remineralized at all. However, there was also an inner layer, immediately adjacent to sound dentine on the floor of the lesion, that could be partially remineralized even though it contained some bacteria, because it still retained some of the original dentine tubule structure. This was called Fig. 6. The periphery of the cavity is prepared to sound dentin or enamel to ensure a good seal. Only a minimal amount of demineralized dentin was removed.
Glass-Ionomer Cements 557Fig. 7. Initial radiographic presentation.the affected layer, and it was suggested that it should not be removed during cavitypreparation as it could be remineralized. However, this suggestion was not widelyaccepted by the profession, because there was no reliable method to differentiatethe infected from affected layers in the dental office. Therefore, there was a need tosimplify this technique further, and the next logical question is: how important is itto differentiate between the two layers so that only the infected layer is removed duringcavity preparation? In a clinical trial conducted by Mertz-Fairhurst and colleagues,23 10 years aftercompletely sealing a lesion where the ‘‘soft, wet, demineralized dentine was left onthe floor of a lesion,’’24 the lesion did not progress or jeopardize the restoration placedabove it. Recently, a review of the literature confirmed that it is acceptable to leave softand wet dentine at the base of cavity preparations, providing a complete seal is estab-lished and maintained.25 There is now evidence suggesting that the partly demineral-ized component of the soft and wet dentine can be remineralized when it comes intocontact with GIC.3 It is a biocompatible material that delivers a long-lasting sealthrough the development of an ion exchange adhesion with both enamel and dentine,with low technique sensitivity. Therefore, the two keys to clinical success when leaving soft dentin behind are, first,to ensure that the tooth does not show signs of irreversible pulpitis and, second, theestablishment of a long-lasting seal.Fig. 8. ‘‘Soft and wet’’ dentine; it is difficult to differentiate between infected and affecteddentine.
558 Ngo Fig. 9. The gingival margin is entirely in dentine; a margin of 2-mm wide was created in sound dentine and the soft dentine, over the pulpal wall, was removed by hand and condi- tioned using 10% polyalkenoic acid. When GIC is placed in direct contact with affected dentine, the migration of apatite- forming elements F and Sr from the GIC to carious dentine can be extensive. In a clin- ical trial study,3 these two elements were found to have accumulated deep into the lesion with the maximum depth reaching over 1.5 mm. The controlling factor was the depth of the lesion and the physical state of the demineralized dentine. The clinical application of the internal remineralization concept is illustrated in the following clinical case. A patient presented with a proximal cavity and reported mild symptoms consistent with reversible pulpitis. There was no evidence of periapical involvement. The initial presentation can be seen in Fig. 4, with only enough enamel removed to gain proper access to the cavity (Fig. 5). Note that the entire enamel margin and dentino-enamel junction have been cleaned to leave 2 mm of sound hard dentine to ensure a seal can be achieved and maintained long-term (Fig. 6). Only hand instrumentation was then used in the removal of the soft dentine immedi- ately above the pulp to minimize the risk of direct pulp exposure. The cavity was then conditioned using 10% polyacrylic acid for 10 seconds. Following conditioning, a small amount of high fluoride-releasing GIC was applied over the soft dentine as a liner. The cavity then was restored with composite resin in the conventional manner. The selection of composite resin for the final restoration was based on the fact that there was sufficient enamel still available right around the periphery of the cavity (see Fig. 6). Fig. 10. A high fluoride-releasing GIC liner is applied to the discolored portion for internal remineralization.
Glass-Ionomer Cements 559Fig. 11. A base of high-strength GIC is placed to ensure a long-lasting seal along thedentine margin. It is suggested that GIC, through its self-adhesive characteristics, will providea complete and long-lasting seal, preventing the ingress of bacteria and potentialnutrients. GIC can be placed in close proximity to the pulp without the risk of inducingirreversible inflammation and the placement of calcium hydroxide is no longer needed,unless there is a direct pulp exposure. Providing that the restoration is completelysealed then there is no risk in leaving the demineralized dentin under the GIC lining.THE SANDWICH TECHNIQUEThis technique uses two different materials for the final restoration, and some clini-cians use the following analogy to describe the rationale for its use; GIC is used asa dentine replacement, while composite resin acts as an enamel replacement. Theindication is badly broken down teeth or when part of the gingival margin is locatedon dentine, because there is doubt on the long-term performance of a dentin adhesivein the absence of enamel.26 The following clinical case is an example of combining theinternal remineralization, to treat carious dentine, and sandwich techniques, to restorethe tooth. This patient presented with a large proximal lesion and reported mild symp-toms over a brief period (Figs. 7 and 8). A clean margin of 2 mm wide was createdusing a round bur, and only hand instruments were used to remove carious dentine.The finished cavity was treated with 10% polyacrylic acid for 10 seconds. Note thatthe enamel transverse ridge was retained so not to weaken the tooth crown (Fig. 9).Fig. 12. Final sandwich restoration.
560 Ngo Fig. 13. Radiograph of final restoration. The discolored dentine was treated with a high F-releasing GIC liner (Fig. 10). A high- strength GIC was laid down as a base in preparation for the composite resin restoration. This was done to ensure a long-lasting seal along the gingival margin (Figs. 11–13), The three practical advantages of this technique are that it Minimizes the risk of pulp exposure Minimizes the number of increments of composite resin to be placed, offering time savings Results in a longlasting seal around the dentine margin. SURFACE PROTECTION FOR ROOT SURFACES IN ELDERLY PATIENTS One of the new challenges clinicians are facing is the maintenance of good oral health in the older patients. Reinhardt predicted that by the year 2030 the number of retained teeth in people living in the United States, aged between 45 to 84, will be approxi- mately 2.2 billion compared with just over 1 billion in 1990. He recognized these teeth will exist in a more hostile oral environment. Root caries can be defined as caries lesions initiated on exposed root surfaces. At an early stage, they are difficult to detect visually, because the first changes are in surface hardness and texture of the affected areas. Unlike enamel lesions, discolor- ation comes much later, and they are usually masked by plaque and inflammation of the surrounding soft tissue. Once established, the lesions can spread incisally by Fig. 14. An exposed and arrested root caries that required protection as the patient could no longer maintain good oral hygiene because of arthritis.
Glass-Ionomer Cements 561Fig. 15. The root surface is now protected with a thin film of GIC.undermining the thin enamel at the CEJ, but more often, they spread below the gumlevel. These lesions quickly become cavitated, because dentin contains much lessmineral than enamel, and more is permeable because of the presence of dentinaltubules. In the following clinical case, GIC was applied as a therapeutic coating toprotect the exposed root surfaces and lesions. The original caries lesion had beenarrested for many years (Fig. 14). This had been achieved with a combination ofgood oral hygiene, use of a high fluoride-containing toothpaste, and daily applicationof a calcium and phosphate-containing paste to saturate the biofilm. The lesion dis-played the three characteristics of a remineralized dentine surface; it was discolored,shiny, and hard. However, with the onset of arthritis, the task of keeping the area cleanbecame too much of a challenge for the patient. After a period of assessment, it wasdecided that the area should be protected with a thin coat of high fluoride-releasingGIC, Fuji Triage (Fuji VII, GC Corp, Tokyo, Japan) (Fig. 15). Being a conventionalGIC, this thin film GIC adheres well to the root surface and acts as a mechanical barrierto protect the area and minimize plaque accumulation. It releases significantly muchmore F than the traditional restorative GICs and if recharged with a daily exposureto fluoridated toothpaste, then the F release can be maintained indefinitely. A thinfilm of half a millimeter or less will allow ions such as calcium and fluoride to crossfrom saliva to the underlying root surface and remineralize it further.SUMMARYGIC is an important tool in the fight against dental caries, and it should be used inconjunction with other traditional tools: It can be thought of as a reservoir of fluoride and other ions in the oral cavity. Externally it can be used as a therapeutic coating to protect the tooth surface against acid and to modulate bacterial activities. It assists in preserving carious dentine at the base of restoration, by delivering F and other apatite-forming ions, and providing a long-lasting seal to both dentine and enamel. GIC can be used as a restorative material, a liner, a base, a luting cement, a fissure sealant, and a surface protectant. The dental profession has come to the realization that to control caries effectively, itis necessary to move from the surgical-only approach to a combined surgical–medicalapproach with special focus on engaging patients in changing their lifestyle. GIC, as
562 Ngo a family of materials, is part of the armamentarium that the clinician has for the management of dental caries, as it can contribute to the surgical and medical manage- ment components. REFERENCES 1. Wilson AD, McLean JW. Glass-ionomer cement. London: Quintessence; 1988. 2. ten Cate JM, van Duinen RN. Hypermineralization of dentinal lesions adjacent to glass-ionomer cement restorations. J Dent Res 1995;74(6):1266–71. 3. Ngo HC, Mount G, McIntyre J, et al. Chemical exchange between glass-ionomer restorations and residual carious dentine in permanent molars: an in vivo study. J Dent 2006;34(8):608–13. 4. Smales RJ, Ngo HC, Yip KH, et al. Clinical effects of glass ionomer restorations on residual carious dentin in primary molars. Am J Dent 2005;18(3):188–93. 5. Mount GJ. Glass ionomers: a review of their current status. Oper Dent 1999;24(2): 115–24. 6. Mount G. An atlas of glass-ionomer cements. A clinician’s guide. London: Martin Dunitz; 2002. 7. Featherstone JD, Shields CP, Khademazad B, et al. Acid reactivity of carbonated apatites with strontium and fluoride substitutions. J Dent Res 1983;62:1049–53. 8. Curzon ME, Adkins BL. Combined effect of trace elements and fluorine on caries. J Dent Res 1970;49:526–9. 9. Wilson AD, Crisp S, Ferner AJ. Reactions in Glass-ionomer Cements: IV. Effect of chelating comonomers on setting behaviour. J Dent 1974;55(3):489–95. 10. Wilson AD. Secondary reactions in glass-ionomer cements. J Mater Sci Lett 1996; 15:275–6. 11. Ngo H, Marino V, Mount GJ. Calcium, strontium, aluminium, sodium, and fluoride release from four glass ionomer cements. J Dent 1998;77:75. 12. Nicholson JW. Chemistry of glass-ionomer cements: a review. Biomaterials 1998; 19:485–94. 13. Okada K, Tosaki S, Hirota K, et al. Surface hardness change of restorative filling materials stored in saliva. Dent Mater 2001;17(1):34–9. 14. Forsten L. Fluoride release and uptake by glass-ionomers and related materials and its clinical effect. Biomaterials 1998;19:503–8. 15. Forsten L. Fluoride release of glass-ionomers. Presented at the 2nd Symposium on Glass Ionomers. Philadelphia, 1994. 16. Cranfield M, Kuhn AT, Winter G. Factors relating to the rates of fluoride release from a glass-ionomer cement. J Dent 1982;10:333–4. 17. Wilson AD, Groffman DM, Kuhn AT. The release of fluoride and other chemical species from a glass-ionomer cement. Biomaterials 1985;6(6):431–3. 18. Hengtrakool C, Pearson GJ, Wilson M. Interaction between GIC and S sanguis biofilms: antibacterial properties and changes of surface hardness. J Dent 2006;34(8):588–97. 19. Beauchamp J, Caufield PW, Crall JP, et al. Evidence-based clinical recommenda- tions for the use of pit-and-fissure sealants: a report of the American Dental Asso- ciation Council on Scientific Affairs. J Am Dent Assoc 2008;139(3):257–68. 20. Arrow P, Riordan PJ. Retention and caries preventive effects of a GIC and a resin- based fissure sealant. Community Dent Oral Epidemiol 1995;23(5):282–5. 21. Fusayama T, Okuse K, Hosoda J. Relationship between hardness, discoloration, and microbial invasion in carious dentin. J Dent Res 1966;45(4):1033–46.
Glass-Ionomer Cements 56322. Massler M. Changing concepts in the treatment of carious lesions. Br Dent J 1967;123(11):547–8.23. Mertz-Fairhurst EJ, Smith CD, Williams JE, et al. Cariostatic and ultraconservative sealed restorations: six-year results. Quintessence Int 1992;23(12):827–38.24. Mertz Fairhurst EJ, Curtis JW, Ergle JW, et al. Ultraconservative and cariostatic sealed restorations: results at year 10. J Am Dent Assoc 1998;129:55–66.25. Kidd EA. How ‘clean’ must a cavity be before restoration? Caries Res 2004;38(3): 305–13.26. De Munck J, Van Meerbeek B, Yoshida Y, et al. Four-year water degradation of total-etch adhesives bonded to dentin. J Dent Res 2003;82(2):136–40.